An in vivo evaluation of bone response to three implant surfaces using a rabbit intramedullary rod model
© Hermida et al; licensee BioMed Central Ltd. 2010
Received: 27 January 2010
Accepted: 16 August 2010
Published: 16 August 2010
Our study was designed to evaluate osseointegration among implants with three surface treatments: plasma-sprayed titanium (P), plasma-sprayed titanium with hydroxyapatite (PHA), and chemical-textured titanium with hydroxyapatite (CHA). Average surface roughness (Ra) was 27 microns for the P group, 17 microns for the PHA group, and 26 microns for the CHA group. Bilateral distal intramedullary implants were placed in the femora of thirty rabbits. Histomorphometry of scanning electron microscopy images was used to analyze the amount of bone around the implants at 6 and 12 weeks after implantation. Greater amounts of osseointegration were observed in the hydroxyapatite-coated groups than in the noncoated group. For all implant surfaces, osseointegration was greater at the diaphyseal level compared to the metaphyseal level. No significant differences were seen in osseointegration between the 6 and 12 week time points. Although the average surface roughness of the P and the CHA groups was similar, osseointegration of the CHA implants was significantly greater. The results of this in vivo lapine study suggest that the presence of an hydroxyapatite coating enhances osseointegration despite similarities in average surface roughness.
Total hip arthroplasty (THA) is a relatively common procedure that typically results in increased comfort, mobility, pain relief, and alleviation of disability. Once thought to be appropriate for patients between 60 and 75 years of age, the age range for primary THA now often includes a substantially younger population [1–4]. The procedure has an excellent clinical outcome and often restores functional capacity to a large degree. However, aseptic loosening of the components continues to limit the longevity of THA, especially in younger more active patients [1–11]. With the increase in life expectancy and the increase in younger patients undergoing primary THA, the need to extend the longevity of THA is essential.
Non-cemented THA offers the potential for integration of the implant surface with the surrounding bone. Hydroxyapatite coatings have proven effective in providing excellent short- and intermediate-term outcomes in terms of fixation, stability, function, and pain relief [12–17]. Hydroxyapatite coatings enhance osteoblast attachment, proliferation, and differentiation (see Beck for review ). While hydroxyapatite is generally considered to be an osteoconductive material, it has occasionally been shown to have osteoinductive properties, which have been attributed to the adsorption of bone morphogenetic proteins .
Osteoblastic activity is modulated by surface roughness and is enhanced when the Ra is between 1 and 7 μm [20, 21]. In addition, surface roughness in vivo is an important factor affecting bone apposition and mechanical strength of the implant-bone interface. Increasing surface roughness by grit-blasting or chemical-etching has been associated with increased osseointegration in a variety of animal models [22–25].
Since hydroxyapatite coating can alter surface roughness, it is important to determine the relative significance of the individual contributions of these factors [22, 26]. For example, superior osseointegration was found in hydroxyapatite-coated trabecular implants in miniature pigs compared to grit-blasted or acid-etched surface . However, the hydroxyapatite-coated implants had a significantly greater Ra. It has not been conclusively shown whether surface roughness or hydroxyapatite coating is the dominant factor affecting in vivo osseointegration. One study concluded that surface roughness contributed more to increased bone apposition rates than hydroxyapatite coating . On the other hand another study found significantly increased bone apposition in hydroxyapatite-coated implants despite comparable surface roughness measures between coated and uncoated implants . We therefore designed a study to investigate the factors contributing to osseointegration in orthopedically relevant surfaces. The study hypothesis was that the addition of a hydroxyapatite coating would enhance osseointegration beyond that provided by change in surface roughness alone.
Thirty adult male New Zealand White rabbits were used in our study. After institutional review board approval, rabbits underwent bilateral femoral intramedullary implantation under general anesthesia. All animals received Buprenorphine 0.03 mg/Kg IM immediately postoperatively, and 0.01 mg/Kg IM every 12 hours for three days. After that any animal demonstrating pain or discomfort received Buprenorphine 0.01 mg/Kg IM. All animals were allowed unrestricted cage activity, and food and water ad libitum. Temperature was maintained at 24°C and humidity at 70%. All rabbits tolerated the anesthesia and surgical procedure uneventfully. Recovery was quick and rabbits were usually ambulating without noticeable limp by postoperative day 7. One rabbit developed intestinal obstruction after ingesting surgical dressing and was euthanized 6 days before schedule. The femora were harvested from this rabbit and included in the SEM analysis.
The femur bone was trimmed above and below the ends of the implant, cleaned of soft-tissue, and fixed in 70% alcohol. The specimen was further dehydrated in absolute alcohol and de-fatted in 50% mixture of ether and acetone before being placed in 100% alcohol again for 12 hours. The specimen was then embedded in methyl methacrylate and transverse sections nominally 1-mm thick cut with a diamond wafering blade at three levels, approximately coinciding with the distal third of the femoral diaphysis, the distal femoral metaphysis, and a level midway between the two. Backscatter electron images were obtained using a scanning electron microscope (JEOL 35, JEOL Ltd, Tokyo, Japan) at 40 × magnifications, 25-KeV beam voltage, and 100 μA emission current at a working distance of 15 mm. Images were of the implant-bone interface were captured around the perimeter of the implant and stored in 8-bit grayscale format at a resolution of 128 pixels per mm (pixel size 7.8 μm).
Automated computerized image analysis was performed on the SEM images using a previously validated approach [22, 29]. A custom script was written (MATLAB, Image Processing Toolbox, MathWorks, Natick, MA). The image was segmented into bone and implant regions based on the trimodal histogram of the image. Images were initially filtered to remove random stray pixels. The image was segmented into three areas represented by: implant pixels (grayscale value between 200 and 255), bone pixels (grayscale value between 80 and 200), and soft-tissue pixels (grayscale value between 0 and 80). An edge detection algorithm was used to detect pixels at the perimeter of the implant and the bone and soft-tissue pixels adjacent to the edge of the implants were counted.
Osseointegration was defined as bone-to-implant contact and calculated as the ratio of the number of bone pixels relative to the total number of pixels (bone + soft tissue) at the perimeter of the implant. Additionally, the relative numbers of bone pixels were measured at varying distances (up to 0.24 mm) radially outward from the perimeter of the implant to detect changes in patterns of bone growth among the different surfaces.
Power analysis determined that a sample size of 10 was adequate to detect differences in osseointegration of greater than 15% among groups with a power greater than 80% and an alpha of 0.05, assuming a standard deviation of up to 11%. Results from four quadrants were averaged to obtain the net osseointegration and presence of bone for each section level.
Multifactorial two-way Analyses of Variance (ANOVA) were performed on mean osseointegration (or presence of bone at 0.03 to 0.24 mm from the implant surface) with surface treatment, time after surgery, and bone section level as the variables. When statistical differences were identified, Tukey post hoc pairwise comparisons were performed. Significant differences were assumed at p ≤ 0.05.
The intramedullary bone response to three titanium surfaces (grit-blasted, porous fiber mesh, and acid-etched) was previously evaluated using the same animal model . In that study, the chemically textured (by acid-etching) surface with a Ra of 18 microns showed higher osseointegration than the grit-blasted surface with and Ra of 6 microns. This study builds on our previous findings by investigating the effect of hydroxyapatite coating on surfaces with different roughness. The PHA and CHA groups had very different Ra values of 17 microns and 26 microns, respectively, yet the osseointegration of each hydroxyapatite-coated surface was comparable, which suggested that the presence of the osteoinductive hydroxyapatite coating had a greater influence on bone growth than the surface roughness. Conversely, the mean Ra values for the P and CHA groups were very similar at 27 microns and 26 microns, respectively. However, the osseointegration and distribution of bone were significantly different between these two groups.
Both surface roughness and hydroxyapatite coating have been shown to increase osseointegration . Some reports have attributed increased osseointegration to surface roughness [23, 31, 32] while other reports to the hydroxyapatite coating [33–36]. Since the hydroxyapatite coating alters the surface roughness, a few studies have attempted to quantify the relative contribution of surface topography versus hydroxyapatite coating. Carlsson et al implanted titanium implants in the upper tibia of osteoarthritic knees of patients scheduled for total knee arthroplasty . The osseointegration reported at 3 months was significantly higher in grit-blasted implants (mean Ra = 3.1) than in implants with a smooth surface (mean Ra = 0.9). This osseointegration was similar to that seen in implants coated with hydroxyapatite (mean Ra = 5.1). However, the sample size studied was small with a large variance in the reported data. In a more controlled canine femoral intramedullary model, Hacking et al determined the relative contributions of surface chemistry and topography on osseointegration . The hydroxyapatite surface of one group of implants was coated with a thin film of titanium, which masked the chemical activity of the hydroxyapatite coat while retaining the topography and surface roughness. Mean osseointegration of hydroxyapatite-coated implants (74%) was higher than the masked hydroxyapatite group (59%) or the grit-blasted group (23%). The relative increase in osseointegration between masked hydroxyapatite implants and grit-blasted implants was larger than the increase in osseointegration between hydroxyapatite-coated and masked hydroxyapatite implants. The authors therefore concluded that surface topography was the dominant factor influencing bone growth.
On the other hand, our study found a stronger correlation between the presence of hydroxyapatite and osseointegration than between surface roughness and osseointegration. In our study, the surface roughness of the implants used ranged from a Ra of 17 to 26 microns. The surface roughness of the implants tested by Carlsson et al and Hacking et al were in the 3 to 6 micron range. It is therefore possible that an interaction effect exists between surface roughness and hydroxyapatite coating on osseointegration. At higher magnitudes of surface roughness, the hydroxyapatite coating may contribute more to osseointegration. The differences in findings underscore the need for additional research to better understand the processes that influence osseointegration.
Osseointegration was significantly higher at the diaphyseal level compared to that at the metaphyseal or intermediate levels. Implant-bone contact as well the type of bone (trabecular versus lamellar) varies along the axial direction. However, the differences in osseointegration along the axial direction were statistically similar between surface treatments. This suggests an absence of interaction effect between surface chemistry and location of implant. The presence of bone in the radial direction also varied by implant surface. Significantly greater bone was present within 0.03 mm of the implant surface in the hydroxyapatite-coated groups. While the SEM could not differentiate between newly deposited bone and pre-existing bone, these differences near the implant-bone surface were likely due to new bone formation.
The similarity in the chemistry of the hydroxyapatite coating with the crystalline phase of bone is believed to be one of the reasons for its excellent biocompatibility and osteoconductive properties. The slow but finite dissolution rate of crystalline hydroxyapatite provides a continuous source of calcium and inorganic phosphate . In our present study, as well as in those reported by others, bone often appears to be directly deposited on the hydroxyapatite coating without any intervening layer of fibrous tissue, the latter being more commonly seen in uncoated titanium surfaces [22, 23, 28, 37]. While hydroxyapatite by itself is considered osteoconductive, in vivo the surface adsorption of proteins (such as bone morphogenetic proteins) may render the surface osteoinductive [38, 39]. In addition, osteoblasts may attach and release active osteoinductive factors. All of these factors combined may be responsible for the enhanced bone response.
Clinical outcomes have substantiated the results of this animal model. Early osseointegration and more stable implant-bone interfaces were seen radiographically. In patients implanted with hydroxyapatite-coated femoral stems, no evidence of mechanical failures or progressive radiolucencies was noted [40, 41]. Evidence exists that hydroxyapatite provides benefits beyond promoting osseointegration and enhancing implant stability. More complete osseointegration may act as a barrier to the migration of polyethylene debris along the bone-implant interface thereby reducing the incidence of osteolysis [9, 10, 42, 43]. Rahbek et al demonstrated that hydroxyapatite effectively prevented particle migration when compared to non-coated grit-blasted titanium alloy implants in a canine femoral model [10, 43, 44]. A ten-year clinical follow up of a hydroxyapatite-coated femoral stem did not find evidence of distal osteolysis despite relatively high polyethylene wear [41, 45]. With current-generation implant designs, short-term stability is no longer a major issue [14, 15, 46, 47]. Longer-term follow up, however, shows polyethylene wear and lysis to be a major concern [48–51]. Measures that directly reduce wear (such as crosslinked polyethylenes and alternative bearing surfaces) have been introduced with some success [52, 53]. However, a higher level of osseointegration is also extremely valuable, because it can reduce the incidence of distal osteolysis, which is one of the primary causes of implant failure [41, 48, 54].
One limitation of the study was the use of only roughness parameter (Ra). Other roughness and surface parameters may also be important in determining potential for osseointegration. Osseointegration was only measured using one histomorphometric parameter (bone-to-implant contact). We did not measure the mechanical strength of the interface that is relevant for hip arthroplasty. However, others have correlated mechanical pull-out strength with the histomorphetric assessment of osseointegration .
Effective osseointegration of noncemented components plays an essential role in implant fixation, long-term stability, and survivorship. Our in vivo study evaluated the bone response to three surfaces, which adds to the body of evidence that is useful for optimizing the osseointegration of implants and enhancing fixation. It is important to identify factors that minimize joint arthroplasty failure and the significant physical and financial costs that failure represents. Finally, clinical outcomes studies are needed to validate the impact of implant surface and related osseointegration on THA outcomes.
- Chmell MJ, Scott RD, Thomas WH, Sledge CB: Total hip arthroplasty with cement for juvenile rheumatoid arthritis. Results at a minimum of ten years in patients less than thirty years old. J Bone Joint Surg Am. 1997, 79: 44-52.PubMedGoogle Scholar
- Garino JP, Steinberg ME: Total hip arthroplasty in patients with avascular necrosis of the femoral head: a 2- to 10-year follow-up. Clin Orthop Relat Res. 1997, 334: 108-115. 10.1097/00003086-199701000-00014.PubMedGoogle Scholar
- Malchau H, Wang YX, Karrholm J, Herberts P: Scandinavian multicenter porous coated anatomic total hip arthroplasty study. Clinical and radiographic results with 7- to 10-year follow-up evaluation. J Arthroplasty. 1997, 12: 133-148. 10.1016/S0883-5403(97)90059-0.View ArticlePubMedGoogle Scholar
- Torchia ME, Klassen RA, Bianco AJ: Total hip arthroplasty with cement in patients less than twenty years old. Long-term results. J Bone Joint Surg Am. 1996, 78: 995-1003. 10.1302/0301-620X78B6.7170.View ArticlePubMedGoogle Scholar
- Berry DJ, Harmsen WS, Ilstrup D, Lewallen DG, Cabanela ME: Survivorship of uncemented proximally porous-coated femoral components. Clin Orthop Relat Res. 1995, 319: 168-177.PubMedGoogle Scholar
- Callaghan JJ, Tooma GS, Olejniczak JP, Goetz DD, Johnston RC: Primary hybrid total hip arthroplasty: an interim followup. Clin Orthop Relat Res. 1996, 333: 118-125. 10.1097/00003086-199612000-00011.PubMedGoogle Scholar
- D'Lima DD, Oishi CS, Petersilge WJ, Colwell CW, Walker RH: 100 cemented versus 100 noncemented stems with comparison of 25 matched pairs. Clin Orthop Relat Res. 1998, 348: 140-148.PubMedGoogle Scholar
- Dickob M, Martini T: The cementless PM hip arthroplasty. Four-to-seven-year results. J Bone Joint Surg Br. 1996, 78: 195-199.PubMedGoogle Scholar
- Engh CA, Culpepper WJ, Engh CA: Long-term results of use of the anatomic medullary locking prosthesis in total hip arthroplasty. J Bone Joint Surg Am. 1997, 79: 177-184. 10.1302/0301-620X.79B2.7640. 2View ArticlePubMedGoogle Scholar
- Petersilge WJ, D'Lima DD, Walker RH, Colwell CW: Prospective study of 100 consecutive Harris-Galante porous total hip arthroplasties. 4- to 8-year follow-up study. J Arthroplasty. 1997, 12: 185-193. 10.1016/S0883-5403(97)90065-6.View ArticlePubMedGoogle Scholar
- Stulberg BN, Singer R, Goldner J, Stulberg J: Uncemented total hip arthroplasty in osteonecrosis: a 2- to 10-year evaluation. Clin Orthop Relat Res. 1997, 334: 116-123. 10.1097/00003086-199701000-00015.PubMedGoogle Scholar
- D'Antonio JA, Capello WN, Crothers OD, Jaffe WL, Manley MT: Early clinical experience with hydroxyapatite-coated femoral implants. J Bone Joint Surg Am. 1992, 74: 995-1008.PubMedGoogle Scholar
- D'Antonio JA, Capello WN, Manley MT: Remodeling of bone around hydroxyapatite-coated femoral stems. J Bone Joint Surg Am. 1996, 78: 1226-1234.PubMedGoogle Scholar
- D'Lima DD, Walker RH, Colwell CW: Omnifit-HA stem in total hip arthroplasty. A 2- to 5-year followup. Clin Orthop Relat Res. 1999, 363: 163-169.PubMedGoogle Scholar
- Geesink RG, Hoefnagels NH: Six-year results of hydroxyapatite-coated total hip replacement. J Bone Joint Surg Br. 1995, 77: 534-547.PubMedGoogle Scholar
- Harris WH: The problem is osteolysis. Clin Orthop Relat Res. 1995, 311: 46-53.PubMedGoogle Scholar
- Kroon PO, Freeman MA: Hydroxyapatite coating of hip prostheses. Effect on migration into the femur. J Bone Joint Surg Br. 1992, 74: 518-522.PubMedGoogle Scholar
- Beck GR: Inorganic phosphate as a signaling molecule in osteoblast differentiation. J Cell Biochem. 2003, 90: 234-243. 10.1002/jcb.10622.View ArticlePubMedGoogle Scholar
- Reddi AH: Morphogenesis and tissue engineering of bone and cartilage: inductive signals, stem cells, and biomimetic biomaterials. Tissue Eng. 2000, 6: 351-359. 10.1089/107632700418074.View ArticlePubMedGoogle Scholar
- Michaels CM, Keller JC, Stanford CM, Solursh M: In vitro cell attachment of osteoblast-like cells to titanium. J Dental Res. 1989, 68: 276-282.Google Scholar
- Curtis A, Clark P: The effects of topographical and mechanical properties of materials on cell behavior. CRC Crit Rev Biocompatibil. 1990, 5: 343-362.Google Scholar
- D'Lima DD, Lemperle SM, Chen PC, Holmes RE, Colwell CW: Bone response to implant surface morphology. J Arthroplasty. 1998, 13: 928-934. 10.1016/S0883-5403(98)90201-7.View ArticlePubMedGoogle Scholar
- Feighan JE, Goldberg VM, Davy D, Parr JA, Stevenson S: The influence of surface-blasting on the incorporation of titanium-alloy implants in a rabbit intramedullary model. J Bone Joint Surg Am. 1995, 77: 1380-1395.PubMedGoogle Scholar
- Wennerberg A, Albrektsson T, Johansson C, Andersson B: Experimental study of turned and grit-blasted screw-shaped implants with special emphasis on effects of blasting material and surface topography. Biomaterials. 1996, 17: 15-22. 10.1016/0142-9612(96)80750-2.View ArticlePubMedGoogle Scholar
- Wong M, Eulenberger J, Schenk R, Hunziker E: Effect of surface topology on the osseointegration of implant materials in trabecular bone. J Biomed Mater Res. 1995, 29: 1567-1575. 10.1002/jbm.820291213.View ArticlePubMedGoogle Scholar
- Hacking SA, Tanzer M, Harvey EJ, Krygier JJ, Bobyn JD: Relative contributions of chemistry and topography to the osseointegration of hydroxyapatite coatings. Clin Orthop Relat Res. 2002, 405: 24-38. 10.1097/00003086-200212000-00004.View ArticlePubMedGoogle Scholar
- Daugaard H, Elmengaard B, Bechtold JE, Jensen T, Soballe K: The effect on bone growth enhancement of implant coatings with hydroxyapatite and collagen deposited electrochemically and by plasma spray. J Biomed Mater Res A. 2010, 92: 913-921.PubMed CentralPubMedGoogle Scholar
- Tisdel CL, Goldberg VM, Parr JA, Bensusan JS, Staikoff LS, Stevenson S: The influence of a hydroxyapatite and tricalcium-phosphate coating on bone growth into titanium fiber-metal implants. J Bone Joint Surg Am. 1994, 76: 159-171.PubMedGoogle Scholar
- Holmes RE, Hagler HK, Coletta CA: Thick-section histometry of porous hydroxyapatite implants using backscattered electron imaging. J Biomed Mater Res. 1987, 21: 731-739. 10.1002/jbm.820210605.View ArticlePubMedGoogle Scholar
- Buser D, Schenk RK, Steinemann S, Fiorellini JP, Fox CH, Stich H: Influence of surface characteristics on bone integration of titanium implants. A histomorphometric study in miniature pigs. J Biomed Mater Res. 1991, 25: 889-902. 10.1002/jbm.820250708.View ArticlePubMedGoogle Scholar
- Gotfredsen K, Berglundh T, Lindhe J: Anchorage of titanium implants with different surface characteristics: an experimental study in rabbits. Clin Implant Dent Relat Res. 2000, 2: 120-128. 10.1111/j.1708-8208.2000.tb00002.x.View ArticlePubMedGoogle Scholar
- Gotfredsen K, Wennerberg A, Johansson C, Skovgaard LT, Hjorting-Hansen E: Anchorage of TiO2-blasted, HA-coated, and machined implants: an experimental study with rabbits. J Biomed Mater Res. 1995, 29: 1223-1231. 10.1002/jbm.820291009.View ArticlePubMedGoogle Scholar
- Darimont GL, Cloots R, Heinen E, Seidel L, Legrand R: In vivo behaviour of hydroxyapatite coatings on titanium implants: a quantitative study in the rabbit. Biomaterials. 2002, 23: 2569-2575. 10.1016/S0142-9612(01)00392-1.View ArticlePubMedGoogle Scholar
- Gottlander M, Albrektsson T, Carlsson LV: A histomorphometric study of unthreaded hydroxyapatite-coated and titanium-coated implants in rabbit bone. Int J Oral Maxillofac Implants. 1992, 7: 485-490.PubMedGoogle Scholar
- Soballe K: Hydroxyapatite ceramic coating for bone implant fixation. Mechanical and histological studies in dogs. Acta Orthop Scand Suppl. 1993, 255: 1-58.View ArticlePubMedGoogle Scholar
- Thomas KA, Kay JF, Cook SD, Jarcho M: The effect of surface macrotexture and hydroxylapatite coating on the mechanical strengths and histologic profiles of titanium implant materials. J Biomed Mater Res. 1987, 21: 1395-1414. 10.1002/jbm.820211205.View ArticlePubMedGoogle Scholar
- Carlsson L, Regner L, Johansson C, Gottlander M, Herberts P: Bone response to hydroxyapatite-coated and commercially pure titanium implants in the human arthritic knee. J Orthop Res. 1994, 12: 274-285. 10.1002/jor.1100120218.View ArticlePubMedGoogle Scholar
- Dong X, Wang Q, Wu T, Pan H: Understanding adsorption-desorption dynamics of BMP-2 on hydroxyapatite (001) surface. Biophys J. 2007, 93: 750-759. 10.1529/biophysj.106.103168.PubMed CentralView ArticlePubMedGoogle Scholar
- Autefage H, Briand-Mesange F, Cazalbou S, Drouet C, Fourmy D, Goncalves S, Salles JP, Combes C, Swider P, Rey C: Adsorption and release of BMP-2 on nanocrystalline apatite-coated and uncoated hydroxyapatite/beta-tricalcium phosphate porous ceramics. J Biomed Mater Res B Appl Biomater. 2009, 91: 706-715.View ArticlePubMedGoogle Scholar
- Hermida JC, Patil S, Colwell CW, D'Lima DD: Bioceramic-implant coatings: correlation between animal and clinical studies. AAOS 72nd Annual Meeting. 2005, 6:Google Scholar
- Lee GY, Srivastava A, D'Lima DD, Pulido PA, Colwell CW: Hydroxyapatite-coated femoral stem survivorship at 10 years. J Arthroplasty. 2005, 20: 57-62. 10.1016/j.arth.2005.04.022.View ArticlePubMedGoogle Scholar
- Bobyn JD, Jacobs JJ, Tanzer M, Urban RM, Aribindi R, Sumner DR, Turner TM, Brooks CE: The susceptibility of smooth implant surfaces to periimplant fibrosis and migration of polyethylene wear debris. Clin Orthop Relat Res. 1995, 311: 21-39.PubMedGoogle Scholar
- McPherson EJ, Dorr LD, Gruen TA, Saberi MT: Hydroxyapatite-coated proximal ingrowth femoral stems. A matched pair control study. Clin Orthop Relat Res. 1995, 315: 223-230.PubMedGoogle Scholar
- Rahbek O, Overgaard S, Lind M, Bendix K, Bunger C, Soballe K: Sealing effect of hydroxyapatite coating on peri-implant migration of particles. An experimental study in dogs. J Bone Joint Surg Br. 2001, 83: 441-447. 10.1302/0301-620X.83B3.10667.View ArticlePubMedGoogle Scholar
- D'Antonio JA, Capello WN, Manley MT, Geesink R: Hydroxyapatite femoral stems for total hip arthroplasty: 10- to 13-year followup. Clin Orthop Relat Res. 2001, 393: 101-111. 10.1097/00003086-200112000-00012.View ArticlePubMedGoogle Scholar
- Capello WN: Hydroxyapatite in total hip arthroplasty: five-year clinical experience. Orthopedics. 1994, 17: 781-792.PubMedGoogle Scholar
- Capello WN, D'Antonio JS, Feinberg JR: Hydroxyapatite-coated stems in patients under 50 years old: clinical radiographic results at five-year minimum follow-up. Orthop Trans. 1995, 19: 399-Google Scholar
- Capello WN, D'Antonio JA, Feinberg JR, Manley MT: Ten-year results with hydroxyapatite-coated total hip femoral components in patients less than fifty years old. A concise follow-up of a previous report. J Bone Joint Surg Am. 2003, 85-A: 885-889.PubMedGoogle Scholar
- Herrera A, Canales V, Anderson J, Garcia-Araujo C, Murcia-Mazon A, Tonino AJ: Seven to 10 years followup of an anatomic hip prosthesis: an international study. Clin Orthop Relat Res. 2004, 423: 129-137. 10.1097/01.blo.0000128973.73132.0b.View ArticlePubMedGoogle Scholar
- Reikeras O, Gunderson RB: Excellent results of HA coating on a grit-blasted stem: 245 patients followed for 8-12 years. Acta Orthop Scand. 2003, 74: 140-145. 10.1080/00016470310013851.View ArticlePubMedGoogle Scholar
- Rokkum M, Brandt M, Bye K, Hetland KR, Waage S, Reigstad R: Polyethylene wear, osteolysis and acetabular loosening with an HA-coated hip prosthesis. A follow-up of 94 consecutive arthroplasties. J Bone Joint Surg Br. 1999, 81: 582-589. 10.1302/0301-620X.81B4.8715.View ArticlePubMedGoogle Scholar
- Digas G, Karrholm J, Thanner J, Malchau H, Herberts P: The Otto Aufranc Award. Highly cross-linked polyethylene in total hip arthroplasty: randomized evaluation of penetration rate in cemented and uncemented sockets using radiostereometric analysis. Clin Orthop Relat Res. 2004, 429: 6-16. 10.1097/01.blo.0000150314.70919.e3.View ArticlePubMedGoogle Scholar
- Muratoglu OK, Bragdon CR, O'Connor DO, Jasty M, Harris WH: A novel method of cross-linking ultra-high-molecular-weight polyethylene to improve wear, reduce oxidation, and retain mechanical properties. Recipient of the 1999 HAP Paul Award. J Arthroplasty. 2001, 16: 149-160. 10.1054/arth.2001.20540.View ArticlePubMedGoogle Scholar
- Geesink RG: Osteoconductive coatings for total joint arthroplasty. Clin Orthop Relat Res. 2002, 395: 53-65. 10.1097/00003086-200202000-00007.View ArticlePubMedGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.